#------------------------------------------------------------------------------
#$Date: 2016-03-26 16:01:19 +0100 (Sat 26 de Mar de 2016) $
#$Revision: 180368 $
#$URL: svn://www.crystallography.net/cod/cif/7/20/37/7203768.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7203768
loop_
_publ_author_name
'León-Reina, Laura'
'Losilla, Enrique R.'
'Martínez-Lara, Maria'
'Bruque, Sebastián'
'Llobet, Anna'
'Sheptyakov, Denis V.'
'Aranda, Miguel A. G.'
_publ_section_title
;
 Interstitial oxygen in oxygen-stoichiometric apatites
;
_journal_issue                   25
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              2489
_journal_paper_doi               10.1039/b503374h
_journal_volume                  15
_journal_year                    2005
_chemical_formula_sum            'La1.56 O4.33 Si'
_chemical_formula_weight         314.21
_chemical_name_systematic        ' ?'
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_audit_creation_date             2005-03-07T16:11
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2005-03-07T16:11 Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            6
_cell_length_a                   9.77167(28)
_cell_length_b                   9.77167
_cell_length_c                   7.21223(21)
_cell_volume                     596.40(2)
_computing_structure_refinement  GSAS
_pd_block_id
2005-03-07T16:11|La933Si6_773K|M.A.G._Aranda|Overall
_pd_phase_name
'from C:/Rietveld/Laura_Rietveld/Sinq_Dic2003/LaSiO/LaSiO_RT/LA933S'
_refine_ls_goodness_of_fit_all   1.95
_refine_ls_matrix_type           full
_refine_ls_number_parameters     87
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.06
_refine_ls_shift/su_mean         0.01
_cod_data_source_file            b503374h.txt
_cod_data_source_block           La933Si6_773K_overall
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (152
times).

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (68 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_cell_volume        596.40027
_cod_database_code               7203768
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 x-y,+x,+z+1/2
3 -y,x-y,+z
4 -x,-y,+z+1/2
5 y-x,-x,+z
6 +y,y-x,+z+1/2
-1 -x,-y,-z
-2 y-x,-x,-z+1/2
-3 +y,y-x,-z
-4 +x,+y,-z+1/2
-5 x-y,+x,-z
-6 -y,x-y,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
LA La1 0.23028(28) -0.01302(33) 0.25 1.0 Uani 0.01139 6
LA La2 0.3333 0.6667 -0.0010(6) 0.841 Uani 0.01897 4
SI SI 0.4002(6) 0.3709(6) 0.25 1.0 Uani 0.01104 6
O O1 0.3228(5) 0.4834(5) 0.25 1.0 Uani 0.03133 6
O O2 0.5923(4) 0.4712(5) 0.25 1.0 Uani 0.02269 6
O O3 0.34242(32) 0.25520(30) 0.07072(27) 1.0 Uani 0.03432 12
O O4 0.0 0.0 0.25 0.946(13) Uani 0.03604 2
O O5 0.01(4) 0.23(4) 0.62(4) 0.0089(22) Uiso 0.03 12
loop_
_atom_type_symbol
_atom_type_number_in_cell
LA 9.364
SI 6.0
O 26.0
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 La1 O2 99.05(14) 5_555 . 3_655 n
O1 La1 O3 148.23(6) 5_555 . 1_555 n
O1 La1 O3 71.56(8) 5_555 . 6_555 n
O1 La1 O3 71.56(8) 5_555 . -3_555 n
O1 La1 O3 148.23(6) 5_555 . -4_556 n
O1 La1 O4 110.34(12) 5_555 . 1_555 n
O1 La1 O5 56(6) 5_555 . 4_554 n
O1 La1 O5 91(7) 5_555 . 5_555 n
O1 La1 O5 154(6) 5_555 . 6_554 n
O1 La1 O5 56(6) 5_555 . -1_556 n
O1 La1 O5 91(7) 5_555 . -2_556 n
O1 La1 O5 154(6) 5_555 . -3_556 n
O2 La1 O3 71.62(12) 3_655 . 1_555 n
O2 La1 O3 83.97(9) 3_655 . 6_555 n
O2 La1 O3 83.97(9) 3_655 . -3_555 n
O2 La1 O3 71.62(12) 3_655 . -4_556 n
O2 La1 O4 150.61(16) 3_655 . 1_555 n
O2 La1 O5 144(6) 3_655 . 4_554 n
O2 La1 O5 92(6) 3_655 . 5_555 n
O2 La1 O5 93(7) 3_655 . 6_554 n
O2 La1 O5 144(6) 3_655 . -1_556 n
O2 La1 O5 92(6) 3_655 . -2_556 n
O2 La1 O5 93(7) 3_655 . -3_556 n
O3 La1 O3 134.55(12) 1_555 . 6_555 n
O3 La1 O3 77.20(5) 1_555 . -3_555 n
O3 La1 O3 59.12(11) 1_555 . -4_556 n
O3 La1 O4 82.93(9) 1_555 . 1_555 n
O3 La1 O5 115(6) 1_555 . 4_554 n
O3 La1 O5 119(7) 1_555 . 5_555 n
O3 La1 O5 23(7) 1_555 . 6_554 n
O3 La1 O5 143(6) 1_555 . -1_556 n
O3 La1 O5 60(7) 1_555 . -2_556 n
O3 La1 O5 57(6) 1_555 . -3_556 n
O3 La1 O3 138.66(16) 6_555 . -3_555 n
O3 La1 O3 77.20(5) 6_555 . -4_556 n
O3 La1 O4 104.89(9) 6_555 . 1_555 n
O3 La1 O5 108(6) 6_555 . 4_554 n
O3 La1 O5 22(7) 6_555 . 5_555 n
O3 La1 O5 133(6) 6_555 . 6_554 n
O3 La1 O5 65(6) 6_555 . -1_556 n
O3 La1 O5 161(7) 6_555 . -2_556 n
O3 La1 O5 87(6) 6_555 . -3_556 n
O3 La1 O3 134.55(12) -3_555 . -4_556 n
O3 La1 O4 104.89(9) -3_555 . 1_555 n
O3 La1 O5 65(6) -3_555 . 4_554 n
O3 La1 O5 161(7) -3_555 . 5_555 n
O3 La1 O5 87(6) -3_555 . 6_554 n
O3 La1 O5 108(6) -3_555 . -1_556 n
O3 La1 O5 22(7) -3_555 . -2_556 n
O3 La1 O5 133(6) -3_555 . -3_556 n
O3 La1 O4 82.93(9) -4_556 . 1_555 n
O3 La1 O5 143(6) -4_556 . 4_554 n
O3 La1 O5 60(7) -4_556 . 5_555 n
O3 La1 O5 57(6) -4_556 . 6_554 n
O3 La1 O5 115(6) -4_556 . -1_556 n
O3 La1 O5 119(7) -4_556 . -2_556 n
O3 La1 O5 23(7) -4_556 . -3_556 n
O4 La1 O5 60(6) 1_555 . 4_554 n
O4 La1 O5 88(6) 1_555 . 5_555 n
O4 La1 O5 61(8) 1_555 . 6_554 n
O4 La1 O5 60(6) 1_555 . -1_556 n
O4 La1 O5 88(6) 1_555 . -2_556 n
O4 La1 O5 61(8) 1_555 . -3_556 n
O5 La1 O5 111(10) 4_554 . 5_555 n
O5 La1 O5 102(13) 4_554 . 6_554 n
O5 La1 O5 46(13) 4_554 . -1_556 n
O5 La1 O5 66(8) 4_554 . -2_556 n
O5 La1 O5 121(11) 4_554 . -3_556 n
O5 La1 O5 112(11) 5_555 . 6_554 n
O5 La1 O5 66(8) 5_555 . -1_556 n
O5 La1 O5 175(12) 5_555 . -2_556 n
O5 La1 O5 66(8) 5_555 . -3_556 n
O5 La1 O5 121(11) 6_554 . -1_556 n
O5 La1 O5 66(8) 6_554 . -2_556 n
O5 La1 O5 46(13) 6_554 . -3_556 n
O5 La1 O5 111(10) -1_556 . -2_556 n
O5 La1 O5 102(13) -1_556 . -3_556 n
O5 La1 O5 112(11) -2_556 . -3_556 n
La2 La2 La2 179.9604 -2_565 . -2_566 n
La2 La2 O1 136.09(10) -2_565 . 1_555 n
La2 La2 O1 136.10(10) -2_565 . 3_665 n
La2 La2 O1 136.13(10) -2_565 . 5_565 n
La2 La2 O2 45.43(10) -2_565 . 2_554 n
La2 La2 O2 45.42(10) -2_565 . 4_664 n
La2 La2 O2 45.42(10) -2_565 . 6_564 n
La2 La2 O1 43.89(10) -2_566 . 1_555 n
La2 La2 O1 43.88(10) -2_566 . 3_665 n
La2 La2 O1 43.90(10) -2_566 . 5_565 n
La2 La2 O2 134.60(10) -2_566 . 2_554 n
La2 La2 O2 134.56(10) -2_566 . 4_664 n
La2 La2 O2 134.58(10) -2_566 . 6_564 n
O1 La2 O1 73.79(15) 1_555 . 3_665 n
O1 La2 O1 73.80(15) 1_555 . 5_565 n
O1 La2 O2 124.40(11) 1_555 . 2_554 n
O1 La2 O2 92.94(8) 1_555 . 4_664 n
O1 La2 O2 154.24(12) 1_555 . 6_564 n
O1 La2 O1 73.81(15) 3_665 . 5_565 n
O1 La2 O2 154.29(12) 3_665 . 2_554 n
O1 La2 O2 124.38(11) 3_665 . 4_664 n
O1 La2 O2 92.96(8) 3_665 . 6_564 n
O1 La2 O2 92.97(8) 5_565 . 2_554 n
O1 La2 O2 154.26(12) 5_565 . 4_664 n
O1 La2 O2 124.42(11) 5_565 . 6_564 n
O2 La2 O2 76.18(16) 2_554 . 4_664 n
O2 La2 O2 76.18(16) 2_554 . 6_564 n
O2 La2 O2 76.17(16) 4_664 . 6_564 n
O1 SI O2 112.4(4) 1_555 . 1_555 n
O1 SI O3 110.86(22) 1_555 . 1_555 n
O1 SI O3 110.86(22) 1_555 . -4_556 n
O1 SI O5 91(11) 1_555 . 6_554 n
O1 SI O5 91(11) 1_555 . -3_556 n
O2 SI O3 108.33(24) 1_555 . 1_555 n
O2 SI O3 108.33(24) 1_555 . -4_556 n
O2 SI O5 142(10) 1_555 . 6_554 n
O2 SI O5 142(10) 1_555 . -3_556 n
O3 SI O3 105.74(33) 1_555 . -4_556 n
O3 SI O5 33(10) 1_555 . 6_554 n
O3 SI O5 90(8) 1_555 . -3_556 n
O3 SI O5 90(8) -4_556 . 6_554 n
O3 SI O5 33(10) -4_556 . -3_556 n
O5 SI O5 63(17) 6_554 . -3_556 n
La1 O1 La2 104.07(12) 3_555 . 1_555 n
La1 O1 La2 104.09(12) 3_555 . -2_566 n
La1 O1 SI 96.28(26) 3_555 . 1_555 n
La2 O1 La2 92.21(19) 1_555 . -2_566 n
La2 O1 SI 128.23(13) 1_555 . 1_555 n
La2 O1 SI 128.22(13) -2_566 . 1_555 n
La1 O2 La2 115.06(11) 5_665 . 2_655 n
La1 O2 La2 115.05(11) 5_665 . -1_665 n
La1 O2 SI 124.79(32) 5_665 . 1_555 n
La2 O2 La2 89.15(21) 2_655 . -1_665 n
La2 O2 SI 103.22(19) 2_655 . 1_555 n
La2 O2 SI 103.23(19) -1_665 . 1_555 n
La1 O3 La1 114.57(14) 1_555 . 2_554 n
La1 O3 SI 97.44(17) 1_555 . 1_555 n
La1 O3 O5 69(17) 1_555 . 6_554 n
La1 O3 SI 142.87(21) 2_554 . 1_555 n
La1 O3 O5 89(15) 2_554 . 6_554 n
SI O3 O5 85(15) 1_555 . 6_554 n
La1 O4 La1 120.0 1_555 . 3_555 n
La1 O4 La1 120.0 1_555 . 5_555 n
La1 O4 La1 120.0 3_555 . 5_555 n
La1 O5 La1 114(11) 2_555 . 3_555 n
La1 O5 La1 109(10) 2_555 . 4_555 n
La1 O5 SI 98(13) 2_555 . 2_555 n
La1 O5 O3 88(20) 2_555 . 2_555 n
La1 O5 La1 114(12) 3_555 . 4_555 n
La1 O5 SI 119(13) 3_555 . 2_555 n
La1 O5 O3 69(14) 3_555 . 2_555 n
La1 O5 SI 101(12) 4_555 . 2_555 n
La1 O5 O3 158(23) 4_555 . 2_555 n
SI O5 O3 62(14) 2_555 . 2_555 n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 La1 4.012(4) . 3_555 n
La1 La1 4.012(4) . 5_555 n
La1 La2 4.1517(30) . 1_545 n
La1 La2 4.1523(30) . -2_556 n
La1 SI 3.256(6) . 1_555 n
La1 SI 3.339(6) . 5_555 n
La1 O1 2.751(6) . 5_555 n
La1 O2 2.531(4) . 3_655 n
La1 O3 2.6211(34) . 1_555 n
La1 O3 2.4722(22) . 6_555 n
La1 O3 2.4722(22) . -3_555 n
La1 O3 2.6211(34) . -4_556 n
La1 O4 2.3165(22) . 1_555 n
La1 O5 2.46(33) . 4_554 n
La1 O5 2.65(26) . 5_555 n
La1 O5 2.45(30) . 6_554 n
La1 O5 2.46(33) . -1_556 n
La1 O5 2.65(26) . -2_556 n
La1 O5 2.45(30) . -3_556 n
La2 La1 4.1517(30) . 1_565 n
La2 La1 4.1523(30) . 3_555 n
La2 La1 4.1526(30) . 5_665 n
La2 La2 3.591(9) . -2_565 n
La2 La2 3.621(9) . -2_566 n
La2 SI 3.331(5) . 2_554 n
La2 SI 3.331(5) . 4_664 n
La2 SI 3.331(5) . 6_564 n
La2 O1 2.513(4) . 1_555 n
La2 O1 2.512(4) . 3_665 n
La2 O1 2.512(4) . 5_565 n
La2 O2 2.558(4) . 2_554 n
La2 O2 2.559(4) . 4_664 n
La2 O2 2.558(4) . 6_564 n
La2 O3 2.9082(28) . -1_665 n
La2 O3 2.9073(28) . -3_565 n
La2 O3 2.9079(28) . -5_555 n
SI La1 3.256(6) . 1_555 n
SI La1 3.339(6) . 3_555 n
SI La2 3.331(5) . 2_655 n
SI La2 3.331(5) . -1_665 n
SI O1 1.616(5) . 1_555 n
SI O2 1.627(5) . 1_555 n
SI O3 1.622(4) . 1_555 n
SI O3 1.622(4) . -4_556 n
SI O5 1.83(28) . 6_554 n
SI O5 1.83(28) . -3_556 n
O1 La1 2.751(6) . 3_555 n
O1 La2 2.513(4) . 1_555 n
O1 La2 2.512(4) . -2_566 n
O1 SI 1.616(5) . 1_555 n
O2 La1 2.531(4) . 5_665 n
O2 La2 2.558(4) . 2_655 n
O2 La2 2.559(4) . -1_665 n
O2 SI 1.627(5) . 1_555 n
O3 La1 2.6211(34) . 1_555 n
O3 La1 2.4722(22) . 2_554 n
O3 La2 2.9082(28) . -1_665 n
O3 SI 1.622(4) . 1_555 n
O3 O5 1.01(32) . 6_554 n
O4 La1 2.3165(22) . 1_555 n
O4 La1 2.3165(22) . 3_555 n
O4 La1 2.3165(22) . 5_555 n
O5 La1 2.45(30) . 2_555 n
O5 La1 2.65(26) . 3_555 n
O5 La1 2.46(33) . 4_555 n
O5 SI 1.83(28) . 2_555 n
O5 O3 1.01(32) . 2_555 n
O5 O5 1.9(5) . -4_557 n
loop_
_pd_block_diffractogram_id
2005-03-07T16:11|La933Si6_773K_H_01|M.A.G._Aranda|hrpt_npd
loop_
_pd_phase_block_id
2005-03-07T16:11|La933Si6_773K_phase1|M.A.G._Aranda||
2005-03-07T16:11|La933Si6_773K_phase2|M.A.G._Aranda||
